Fig S6. characteristics of PSCs based on Polymer : PC71BM with and without 3% DIO additive. J-V Table S4. Photovoltaic properties of PSCs made from chloroform solution with a ITO/PEDOT:PSS/polymer:ITIC (1:1, w/w)/LiF/Al device structure measured under AM 1.5G illumination (100 mW cm-2); Acceptor FF PCE Voc Jsc Donor (V) (mA cm-2) (%) (%) 0.73 2.64 63.3 1.22 Ran-BT (0.63a) (4.97a) (60.5a) (1.89a) 0.66 1.46 50.0 0.48 Reg-BT (0.58a) (3.42a) (56.2a) (1.12a) PC71BM 0.74 1.93 55.3 0.79 Ran-TT (0.64a) (4.22a) (64.0a) (1.73a) 0.66 1.44 48.8 0.47 Reg-TT (0.57a) (3.11a) (51.2a) (0.90a) a With 3% DIO Properties of HOD and EOD
Fig S6. J-V characteristics of PSCs based on Polymer : PC71BM with and without 3% DIO additive. Table S4. Photovoltaic properties of PSCs made from chloroform solution with a ITO/PEDOT:PSS/polymer:ITIC (1:1, w/w)/LiF/Al device structure measured under AM 1.5G illumination (100 mW cm-2); Acceptor Donor Voc (V) Jsc (mA cm-2) FF (%) PCE (%) PC71BM Ran-BT 0.73 (0.63a) 2.64 (4.97a) 63.3 (60.5a) 1.22 (1.89a) Reg-BT 0.66 (0.58a) 1.46 (3.42a) 50.0 (56.2a) 0.48 (1.12a) Ran-TT 0.74 (0.64a) 1.93 (4.22a) 55.3 (64.0a) 0.79 (1.73a) Reg-TT 0.66 (0.57a) 1.44 (3.11a) 48.8 (51.2a) 0.47 (0.90a) a With 3% DIO Properties of HOD and EOD
1-s2.0-S0032386118304233-mmc1.docx